Copper Chalcogenide Semiconductors for Photovoltaic Applications Brian Evanko Materials 286G 2 June 2014
Thin Film Solar cells • Thin film solar cell semiconductors have very high absorption coefficients and are manufactured with much less material. • Efficiency is lower than crystalline Si, but so is $/W. • P-type absorber layer: • Eg from 1 to 1.5 eV • Absorption coefficient > 104 cm-1 Al Hicks. Driving Solar Innovations from Laboratory to Marketplace. NREL Continuum. 2014. www.nrel.gov/continuum/spectrum/photovoltaics.cfm
Copper Chalcogenides Y. Zhao and C. Burda, “Development of plasmonic semiconductor nanomaterials with copper chalcogenides for a future with sustainable energy materials,” Energy Environ. Sci., vol. 5, no. 2, p. 5564, 2012. CZTS CIGS Cu2S
Outline • Binary Cu2S • Early Cu2S/CdScells • Material instability • Ternary (I-III-VI2) materials • Copper indium selenide(CIS) • Copper gallium selenide (CGS) and CIGS • Derivation of chalcopyrite from zinc blende • Quaternary (I2-II-IV-VI4) materials • Copper zinc tin sulfide (CZTS) and selenide (CZTSe) • Derivation of kesterite from chalcopyrite
Cuprous Sulfide (Cu2S) • P-type with 1.2 eV band gap • CdS/Cu2S heterojunctioncells have efficiencies of10% • Most common synthesis method is cation exchange by dipping CdS film into CuCl J. Tang, Z. Huo, Sarah Brittman, HanweiGao and Peidong Yang . “Solution-processed core–shell nanowires for efficient photovoltaic cells.” Nature Nanotechnology6, 568–572 (2011).
Structure of CuxS Phases Q. Xu, B. Huang, Y. Zhao, Y. Yan, R. Noufi, and S.-H. Wei, “Crystal and electronic structures of CuxS solar cell absorbers,” Appl. Phys. Lett., vol. 100, no. 6, p. 061906, 2012.
Analysis of CuxS Synthesizing and identifying phase-pure materials is difficult Digenite Y. Zhao and C. Burda, “Development of plasmonic semiconductor nanomaterials with copper chalcogenides for a future with sustainable energy materials,” Energy Environ. Sci., vol. 5, no. 2, p. 5564, 2012. R. Blachnik and A. Muller, “The formation of Cu2S from the elements I. Copper used in form of powders,” Thermochim. Acta, vol. 361, pp. 31–52, 2000
Copper Indium Selenide • CuInSe2 (CIS) has Eg= 1 eV • I-III-VI2 copper chalcogenide semiconductor with chalcopyrite structure • Band gap is tunable from 1 eV – 1.7 eV by forming solid solution with CuGaSe2 (CGS) • CuInxGa1-xSe2 (CIGS) now rivals CdTe with 20% solar energy conversion efficiency
Chalcopyrite Crystal Structure Zinc Blende Chalcopyrite en.wikipedia.org/wiki/File:Sphalerite-unit-cell-3D-balls.png and en.wikipedia.org/wiki/File:Chalcopyrite-unit-cell-3D-balls.png
Density of States • Top of the valence band is a hybridization of Cu d-states and Se p-states. • VB has antibonding character. Energy is increased by repulsive p-d interactions, lowering the band gap. • This behavior is different than many semiconductors, and attributed to the high-energy Cu d-electrons S. Siebentritt, M. Igalson, C. Persson, and S. Lany, “The electronic structure of chalcopyrites-bands, point defects and grain boundaries,” Prog. Photovoltaics Res. Appl., vol. 18, no. 6, pp. 390–410, Sep. 2010.
Copper Zinc Tin Sulfide • Cu2ZnSnS4 (CZTS) has Eg=1.5 eV • I2-II-IV-VI4copper chalcogenide semiconductor with kesterite structure • Band gap is tunable from 1 eV – 1.5 eV by forming solid solution with Cu2ZnSnSe4 to get Cu2ZnSn(SxSe1-x)4(CZTSSe) • CZTSSe has surpassed 10% solar energy conversion efficiency • Earth abundant materials
Kesterite Crystal Structure J. Paier, R. Asahi, A. Nagoya, and G. Kresse, “Cu2ZnSnS4 as a potential photovoltaic material: A hybrid Hartree-Fock density functional theory study,” Phys. Rev. B, vol. 79, no. 11, pp. 115–126, Mar. 2009. Chalcopyrite Kesterite
Density of States For CZTS and CZTSe, the top of the valence band is a hybridization of Cu d-states and chalcogenp-states, similar to CIGS. C. Persson, “Electronic and optical properties of Cu2ZnSnS4 and Cu2ZnSnSe4,” J. Appl. Phys., vol. 107, no. 5, p. 053710, 2010. Kesterite Cu2ZnSnSe4 Kesterite Cu2ZnSnS4
CZTS Electronic Structure Molecular interaction and band diagrams for CZTS • J. Paier, R. Asahi, A. Nagoya, and G. Kresse, “Cu2ZnSnS4 as a potential photovoltaic material: A hybrid Hartree-Fock density functional theory study,” Phys. Rev. B, vol. 79, no. 11, pp. 115–126, Mar. 2009.
Performance Copper chalcogenides are well represented in the categories of thin-film and emerging photovoltaics. Research Cell Efficiency Records. National Renewable Energy Laboratory. 2014. www.nrel.gov/ncpv/
Summary • Cu2S showed early promise but is limited by low stability. • CISe has a chalcopyrite structure and a low band gap • Eg can be increased by incorporating gallium. • CZTS has a kesterite structure and a high band gap • Eg can be decreased by incorporating selenium • Chalcopyrite and kesterite are derived from zinc blende I. Repins, N. Vora, C. Beall, S. Wei, Y. Yan, M. Romero, G. Teeter, H. Du, B. To, and M. Young, “Kesterites and Chalcopyrites : A Comparison of Close Cousins,” in Materials Research Society Spring Meeting, 2011, no. May.